| ||Format||Pages||Price|| |
|5||$43.00||  ADD TO CART|
|Hardcopy (shipping and handling)||5||$43.00||  ADD TO CART|
Significance and Use
4.1 Contaminants may enter the package through leaks. Alternatively, product may be lost from the package through leaks. These leaks are frequently found at seals between package components of the same or dissimilar materials.
4.2 Ingress or egress of gas or moisture through leaks in a package can also degrade sensitive contents.
4.3 There is no general agreement concerning the level of leakage that is likely to be deleterious to a particular package. However, since these tests are designed to detect leakage, components that exhibit any indication of leakage may be rejected.
4.4 These procedures are suitable for use to verify and locate leakage sites. They are not quantitative. No indication of leak size can be inferred from the test. Therefore, this method is employed as a go/no-go test.
4.5 This test is destructive. All package or component test samples exposed to dye penetration testing may not be used for final product packaging.
1.1 This test method defines a procedure that will detect and locate a leak equal to or greater than a channel formed by a 50 µm [0.002 in.] wire in the edge seals of a nonporous package. A dye penetrant solution is applied locally to the seal edge to be tested for leaks. After contact with the dye penetrant for a minimum specified time, the package is visually inspected for dye penetration or, preferably, the seal edge is placed against an absorbent surface and the surface inspected for staining from the dye.
1.2 This test method is used for both transparent and opaque nonporous surfaces.
1.3 This test method requires that the dye penetrant have good contrast to the materials being tested and/or the absorbent surface.
1.4 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E171 Practice for Conditioning and Testing Flexible Barrier Packaging
ICS Number Code 55.040 (Packaging materials and accessories)
UNSPSC Code 24120000(Packaging materials)
ASTM F3039-13, Standard Test Method for Detecting Leaks in Nonporous Packaging or Flexible Barrier Materials by Dye Penetration, ASTM International, West Conshohocken, PA, 2013, www.astm.orgBack to Top